Ionic conductivity values of MG-based polymer electrolytes incorporated with salt, plasticizer and filler.
Elastomers refer to natural or synthetic amorphous polymers which exhibit elastic properties of rubber. Elastomers are able to deform under stress and return to its original state upon removal of stress. As elastomers exhibit glass transition temperatures (Tg) below room temperature (r.t.), elastomers are soft and rubbery at r.t, and segmental motion exists. Elastomers, which contain polar atoms, such as oxygen (O), fluorine (F) and nitrogen (N), can be suitably employed as matrices in polymer electrolytes (PEs). The electronegative atoms serve as electron donors and are able to coordinate with cations from inorganic salts to form a complex. Among elastomers that have been employed in PEs include modified and copolymerised polyisoprene or natural rubber, polyurethanes, and polysiloxanes. This chapter focuses on the progress of natural rubber and its derivatives in the field of polymer electrolytes, and discussesc their interactions with other components of the PEs and ion conduction. Area percentage of ionic species, as well as ion transport parameters, such as number density, mobility and diffusion coefficient of lithium ions as obtained from deconvolution of infrared (IR) spectra, are also discussed in this book chapter.
- polymer electrolytes
- natural rubber
- ion transport
Polymer electrolytes (PEs) are ionic conductors, which consist of inorganic salts dissolved in polymer(s). Since the discovery of PEs by Fenton et al. , PEs are widely investigated by researchers with the aim to design flexible, light-weight, and safer solid-state ionic conductors as alternatives to the commercial leakage-prone liquid electrolytes. Excellent performing polymer electrolytes are aimed to be employed in electrochemical devices, such as fuel cells, rechargeable batteries, solar cells, sensors, supercapacitors, and electrochromic devices. The main components of a basic PE system include a polymer matrix, which serves as medium to hold the conducting ions; an inorganic salt, which acts as source of ions or charge carriers; and a solvent, which helps to dissolve the polymer and dissociate the ions from the salt. It is widely known that ion conduction occurs predominantly in the amorphous regions of the polymer electrolyte . Hence, elastomers are suitable media for ion conduction to occur as their low glass transition temperature (
Apart from possessing polar electron donating atoms, an elastomer has to meet certain criteria for it to be suitable for use as a polymer matrix in PEs. The elastomer also has to exhibit desirable mechanical and thermal properties, which enables it to be applicable in electrochemical devices. Complexation of cations to the polymer matrices is labile to allow ions to be transported via ion hopping and polymer segmental motion. Elastomers that have been used as polymer matrix in PEs are modified and copolymerised polyisoprene or natural rubber, polyurethanes, and polysiloxanes, which will be described briefly below. The chemical structures of natural rubber, polyurethane, and polysiloxane are depicted in Figure 1.
Natural rubber is widely used in many applications due to its characteristics such as flexibility, high tensile strength, being waterproof, and its availability from the rubber tree. Among applications that utilise natural rubber include tyres for vehicles, gloves and other industrial, consumer, and medical products. One of the reasons that sets natural rubber apart from the other elastomers as a preferred polymer matrix in polymer electrolytes mentioned in this chapter is that it is a natural or biopolymer, hence its sustainability and lower cost.
One setback of natural rubber is that it does not contain polar atoms that can complex with cations from salt. Hence, researchers have carried out modifications such as grafting and epoxidation to incorporate polymers possessing polar groups to allow ion transport. The use of natural rubber (
Polyurethane is known for its high tensile strength and elasticity, which can be found in gaskets, cushioning, wheels and tyres for roller coasters and escalators, hoses, surface coatings and sealants, and biomedical devices. The uniqueness of polyurethane is found in its structure which is made up of alternating soft segments and hard segments connected by urethane linkages (NH─C═O─O). The soft segment of polyurethane is made up of long, flexible chains contributed by polyols, while the hard segment is made up of hydrogen bonded C═O and N─H groups contributed by isocyanates to form rigid physically cross-linked domains distributed in the soft segment matrix. In short, the soft segment provides medium for ion conduction, while the hard segment acts as reinforcing filler to provide dimensional stability. The O atoms in the soft segment of the polymer can coordinate with cations from salt to produce ion conduction. Its good adhesive property also allows good electrolyte-electrode contact during electrochemical device fabrication. Polyurethane-based polymer electrolytes have been reported to exhibit conductivity (
Another elastomer that has been employed as polymer, matrix is polysiloxane, also known as silicones. Polysiloxanes are commonly found in silicone oil, grease, rubber, resin, plastics, and so on. Polysiloxanes are inorganic comb polymers, which are composed of substituents connected to the silicon with alternating silicon and oxygen atoms. This group of polymer is known to exhibit very low
In this chapter, we focus on natural rubber–based polymer matrices, that is, modified natural rubber, namely PMMA-grafted natural rubber (MG) in polymer electrolytes. The conductivity, interactions between components, crystallinity as well as glass transition temperature of MG-based polymer electrolytes containing inorganic salt, plasticizer, and filler are discussed.
2. PMMA-grafted natural rubber (MG)
PMMA is a promising candidate as a polymer matrix which has been widely studied in polymer electrolytes since 1985 . Advantages of PMMA include its high stability towards lithium electrode, which translates to higher life cycle in lithium batteries. Being an amorphous polymer, PMMA contains oxygen atoms in the carbonyl (C═O) and (C─O─C) groups, which can act as electron donor to complex with cations from salt. The presence of polar groups in PMMA in addition to its amorphous nature, high transparency, weatherability and good dimensional stability makes it suitable to be grafted with natural rubber. However, PMMA suffer from limitations in terms of mechanical strength and tends to be brittle . Hence, combining the conducting ability of PMMA and the elasticity of natural rubber would counteract the limitations of the two polymers. The ability of PMMA to transport ions along its polymer chains combined with the resilience and flexibility of natural rubber allows PMMA-grafted natural rubber (MG), such as MG30 and MG49, to be employed as polymer matrices for ionic conductors. Figure 2 illustrates the chemical structure of MG polymer matrix.
The chemical structure of MG30 and MG49 are similar and differs in the composition of PMMA which is grafted on natural rubber, where 30 and 49 represent the percentage of the methacrylate polymer present. Research on MG49 as a polymer matrix in polymer electrolytes has received more attention as compared to MG30, probably due to the higher amount of PMMA, and hence, more electron donors in the former are available for complexation with cations from salt.
2.1. MG-based polymer electrolytes incorporated with inorganic salts
MG-based PEs are easily prepared into films by dissolving MG polymer matrices in either toluene [21, 22] or tetrahydrofuran [5, 23] together with inorganic salt(s), and then solution casted to dry. In order to ease dissolution, the MG polymers are usually sliced into smaller pieces prior to use.
The ambient ionic conductivity of MG30 without addition of salt was reported to be in the order between 10−11 and 10−10 S cm−1 [5, 23], which is comparable to that of other synthetic polymers. Examples of salts added into MG30 and/or MG49 are lithium triflate (LiCF3SO3) [4, 5], lithium perchlorate (LiClO4) , lithium tetrafluoroborate (LiBF4) , and ammonium triflate (NH4CF3SO3) , which provide ions for conduction to occur in the polymer matrix system.
Upon the incorporation of salt in MG polymer matrices, maximum conductivity is usually achieved with salt contents in the range of 15–35 wt.%. The increase in conductivity before the maximum point has been attributed to the increase in free ions  resulting from the salt dissociation. This is achieved by the complexation of salt cation with the electron donor atoms in the polymer matrix or solvent, while the separated anions will move freely around in the polymer. With increasing salt content, the amount of available complexation sites on the polymer matrices will be saturated, and hence, the cations will tend to associate with anions of salt to form less mobile ion pairs or ion aggregates [5, 23]. The reduction in free ions in combination with other factors, such as lower ion mobility and increased viscosity, can be used to explain the drop in the ionic conductivity beyond the maximum point .
Yap et al.  reported the best room temperature conductivity of 1.7 µS cm−1 obtained in MG30 sample containing 30 wt.% LiCF3SO3. The ion mechanism was found to obey the Arrhenius law, which suggested that ion transport occurs predominantly through ion hopping. The conductivity trend is in agreement with the trends of activation energy (
The conductivity values of MG30- and MG49-based polymer electrolytes are listed in Table 1. Most MG-salt complexes reported an ambient ionic conductivity around 10−8 to 10−7 S cm−1, which is considered insufficient for application in electrochemical devices.
|Composition (wt.%)||Ambient conductivity, ||Reference|
|MG30: LiCF3SO3 (70:30)||1.7 × 10−6|||
|MG30:LiCF3SO3 (65:35)||a8.4 × 10−4|||
|MG30:LiCF3SO3:EC (15:9:76)||a9.0 × 10−3|||
|MG30:LiCF3SO3:PC (26:14:60)||a3.1 × 10−3|||
|MG30:LiCF3SO3:PEG200 (63:27:10)||3.7 × 10−4|||
|MG30:NH4CF3SO3 (65:35)||2.0 × 10−4|||
|MG30:NH4CF3SO3:EC (32.5:17.5:50)||8.9 × 10−4|||
|MG30:LiCF3SO3:SiO2 (60:33:7)||≈2.3 × 10−4|||
|MG30:LiCF3SO3:SiO2:DMC (18:9.9:2.1:70)||≈3.5 × 10−4|||
|MG30:LiCF3SO3:Al2O3 (59.8:32.2:8)||1.1 × 10−6|||
|MG49:LiBF4 (80:20)||2.3 × 10−7||[35, 36]|
|MG49:LiClO4 (85:15)||4.0 × 10−8|||
|MG49:LiClO4:TiO2 (72:18:10)||3.5 × 10−6|||
|MG49:LiClO4:TiO2:EC (49:14:7:30)||1.1 × 10−3|||
|MG49:NH4CF3SO3-PC (3:97)||1.2 × 10−2|||
|MG49:NH4CF3SO3-PC:SiO2 (2.8:89.2:8.0)||7.6 × 10−3|||
|MG49:LiClO4: [HNO3-THF-TiO2-SiO2] (69:23:8)||5.86 × 10−7|||
2.2. MG-based polymer electrolytes incorporated with plasticizers
Plasticization is a common method used by researchers to enhance the ionic conductivity of polymer electrolytes. This is because plasticizers can increase the amorphousness of the polymer, and enhance polymer segmental motion and ion mobility . The high dielectric constant of plasticizers can also help to dissociate the salt into free ions and prevent ion association . Overall, plasticizer addition helps to improve the ionic conductivity of polymer electrolytes, which is an important factor that influences the device performance.
As mentioned earlier, most MG-based solid polymer electrolytes suffer from low conductivity (
One of the pioneering works on MG-based polymer electrolytes is by Kumutha et al.  who investigated on MG30-LiCF3SO3-EC-Al2SiO5 system. Results from infrared (IR) and differential scanning calorimetry (DSC) studies showed no distinct change in their wavenumbers and
In separate works, Ali and co-workers [4, 23] investigated on MG30-LiCF3SO3-EC and MG30-LiCF3SO3-PC systems. The ionic conductivity increased from 8.4 × 10−4 S cm−1 to achieve maximum conductivity at 9.0 × 10−3 S cm−1 for the EC system, and 3.1 × 10−3 S cm−1 for the system with PC on incorporation of 76 wt.% EC and 61 wt.% PC. For the MG30-LiCF3SO3-PC system, Ali et al.  reported that the sample containing 61 wt.% PC lost its dimensional stability despite exhibiting the best conductivity in the polymer electrolyte system. Increase in conductivity is attributed to several factors, namely increased polymer-cation interaction, high dielectric constant (
Zaki et al.  achieved considerably high ionic conductivity of 2.0 × 10−4 S cm−1 for MG30-NH4LiCF3SO3 (65:35) sample. Ionic conductivity increased to 8.9 × 10−4 S cm−1 upon introduction of 50 wt.% EC. The authors attributed the conductivity enhancement to the high dielectric constant of EC, which helped to dissociate the salt and prevent ion association. Ion conduction was found to follow Vogel-Tammann-Fulcher (VTF) behaviour, whereby ion transport occurs in the amorphous phase via polymer segmental motion. Results from XRD showed reduction in crystallinity from the gradual broadening of amorphous hump located from 2
In the work of Yap et al. , PEG was added into MG30-LiCF3SO3 system. Conductivity improved from 1.7 × 10−6 S cm−1 to a maximum value at 3.7 × 10−4 S cm−1, and this was exhibited in the sample containing 10 wt.% PEG. X-ray diffraction (XRD) analysis confirmed the sample to exhibit the lowest degree of crystallinity.
2.3. MG-based polymer electrolytes incorporated with fillers and other additives
Although polymer electrolytes added with plasticizer exhibit conductivity enhancement, they suffer from low mechanical stability . Hence, researchers have attempted using inorganic fillers to improve the physical and mechanical properties of polymer electrolytes. For MG-based polymer electrolytes, fillers that have been reported are aluminium silicate (Al2SiO5) , silica (SiO2) [28, 30], alumina (Al2O3)  and titania-silica (TiO2-SiO2) , which are all passive fillers, and therefore do not participate directly in the Li+ ion transport process. Filler-added polymer electrolytes are known as composite polymer electrolytes (CPEs).
In the work of Hashim et al. , SiO2 filler was incorporated into MG30-LiCF3SO3, followed by the addition of dimethyl carbonate (DMC) plasticizer. The ionic conductivity initially increased from ≈6.0 × 10−5 S cm−1 to 2.3 × 10−4 S cm−1 upon addition of 7 wt.% SiO2. The rise in conductivity is attributed to the formation of conducting pathways for ion transport. Decreased conductivity above 7 wt.% SiO2 was caused by the blocking effect of the nanofillers. After that, the authors managed to further enhance the conductivity value to ≈3.5 × 10−4 S cm−1 with addition of 7 wt.% DMC. The DMC plasticizer enhanced polymer segmental motion.
MG49-NH4CF3SO3-PC-SiO2 CPE system was reported by Kamisan et al. . The authors first determined the best conducting NH4CF3SO3 molarity in PC at 0.7 M. Gel polymer electrolyte containing 3 wt.% MG49 in the NH4CF3SO3-PC liquid electrolyte exhibited high conductivity in the order of 10−2 S cm−1. However, they lacked mechanical stability due to the high amount of liquid electrolyte. The addition of SiO2 initially decreased the conductivity to 10−3 S cm−1, but increased to achieve two maxima at 1.2 × 10−2 S cm−1 (3 wt.% SiO2) and 7.6 10−3 S cm−1 (8 wt.% SiO2). The activation energy values calculated from the Arrhenius equation displayed two minima at 0.11 and 0.12 eV for samples with 3 and 8 wt.% SiO2 content, respectively. The CPE viscosity increased from 10.0 to 68.2 cP upon addition of 8 wt.% SiO2, which authors took as indication of increased mechanical stability.
Kang and co-workers  incorporated fixed amount of TiO2-SiO2 filler into MG49-LiClO4 system containing different solvents, that is, HNO3-THF and CIHNO2-THF. The conductivities of both MG49-LiClO4-HNO3-THF-TiO2-SiO2 and MG49-LiClO4-CIHNO2-THF-TiO2-SiO2 systems increased from 1.2 × 10−4 S cm−1 to achieve a maximum at 5.9 × 10−7 S cm−1 and 4.8 × 10−7 S cm−1, respectively, upon incorporation of 25 wt.% LiClO4, before decreasing at higher salt contents. Above 25 wt.% LiClO4, the ion transport process is hindered by ionic aggregation and the formation of transient cross-links. The two different polymer electrolyte systems exhibited different ion conduction behaviors: the system containing HNO3-THF followed the Arrhenius rule, whereby ion transport occurs by ion hopping, whereas the CIHNO2-THF system obeyed VTF rule, which indicates polymer segmental relaxation. Both polymer electrolyte systems are thermally stable up to around 270–290°C.
Thermal oxidation of MG-based electrolytes has also been a subject of study. Aging of polymers, which in this case is natural rubber, is a topic of concern as the unsaturated hydrocarbons will degrade on exposure to oxygen and elevated temperatures. Consequently, the physical, electrical, mechanical, and other characteristics of PEs will deteriorate upon aging. Aziz and Ali  studied the effect of varied contents of an antioxidant, N-(1,3-dimethylbutyl)-N′-phenyl-p-phenylenediamine (6PPD) on the thermal oxidation resistance of MG30. Using IR analysis, the absorbance/intensity ratio of the C═O band at 1726 cm−1 to the ═C─H band located at ≈835 cm−1 of different MG30-6PPD samples were calculated to determine the degree of oxidation [33, 34]. Only the sample with 0.5 wt.% 6PPD displayed anti-oxidation effects as the intensity ratio of the bands 1726 cm−1:835 cm−1 decreased. At higher contents of 6PPD (1, 2, 4, 6 and 8 wt.%), no anti-oxidation effect was observed. However, the MG30 sample containing 0.5 wt.% 6PPD with the best anti-oxidation effect exhibited a lower ambient conductivity of 5.50 × 10−6 S cm−1 than the untreated sample which had conductivity of 3.10 × 10−5 S cm−1. The authors suggested incorporating plasticizer to increase the conductivity of MG30-6PPD sample in the future.
2.4. Blends of PMMA-grafted natural rubber
In order to improve the properties of MG30- and MG49-based polymer electrolytes, researchers have attempted blending of the MG polymer matrices with other polymers. MG polymer matrices were simply mixed together with another polymer to produce polymer blend(s) which possess properties that are superior than individual polymers. MG49 has been blended with PMMA , PEO , PVdF-HFP , and PVdF . The chemical structures of PMMA, PEO, PVdF-HFP, and PVdF are shown in Figure 4.
Ahmad et al.  found improvement in the conductivity of MG49 with and without LiBF4 salt upon blending of the polymer with 50 wt.% PMMA. Pure MG49 exhibited ambient conductivity of 1.0 × 10−12 S cm−1, whereas pure MG49-PMMA blend possessed conductivity of 1.7 × 10−12 S cm−1. Upon incorporation of LiBF4, MG49-LiBF4 and MG49-PMMA-LiBF4 samples exhibited maximum conductivity of 2.3 × 10−7 S cm−1 (at 20 wt.%) and 8.3 × 10−6 S cm−1 (at 25 wt.%), respectively. The more superior conductivity in the polymer blend electrolyte is attributed to the higher ratio of number of oxygen atoms to lithium ion [O:Li+] of 5:1 as compared to 8:1 in single polymer electrolyte system. Morphology study by scanning electron microscopy (SEM) revealed homogenous surface in MG49 and MG49-PMMA films with no phase separation. The changes in the structure of MG49 upon blending with PMMA indicated that intermolecular interactions between the two polymers have occurred. Crystals of LiBF4 in MG49 sample added with 25 wt.% of the salt were reported due to salt aggregation above its optimum concentration, which explained the drop in conductivity above 20 wt.% LiBF4.
A polymer blend system that comprised PEO-MG49 with varied wt.% PEO was reported by . Photograph of the PEO:MG49 with wt.% ratio of 60:40 showed a more homogeneous surface and free-standing film, as compared to other wt. ratios (80:20, 20:80, 40:60) which were not homogeneous. From SEM analyses, MG49 film was smooth due to its amorphous characteristic, while PEO film displayed rough surface attributable to its crystalline nature. Upon blending between the two polymers, homogeneous surface was reported for PEO-MG49 sample, whereby the two polymers were well distributed. With increasing addition of LiClO4, the co-continuous phase appeared smoother and increased in pore size. Addition of PEO into MG49 was reported to improve the conductivity by two orders of magnitude. The PEO-MG49-LiClO4 samples exhibited conductivity that was also higher than PEO-LiClO4 sample (
|Polymer electrolyte composition (wt.%)||Ambient conductivity (S cm−1)||Reference|
|MG49:PMMA (70:30)||1.1 × 10−12|||
|4.1 × 10−12|||
|MG49:PMMA:LiClO4 (52.5:22.5:25)||1.5 × 10−8|||
|MG49:PMMA:LiBF4 (52.5:22.5:25)||8.6 × 10−6|||
|PEO:MG49 (60:40)||4.0 × 10−9|||
|PEO:MG49: LiClO4 (51:34:15)||8.0 × 10−6|||
|PVdF-HFP: MG49: LiBF4 (49:21:30)||2.8 × 10−4|||
|PVdF-MG49:LiTCF3SO3 (70:30)||3.3 × 10−4|||
Su’ait and co-workers  blended MG49 with PMMA in the wt.% ratio of 70 to 30, and incorporated the polymer matrix with different lithium salts, namely LiClO4 and LiBF4. The best conductivity was obtained upon addition of 25 wt.% salt in both PE systems. The PE containing LiBF4 exhibited higher conductivity (
Among the polymer-blend electrolyte systems listed in Table 2, fluorine (F)-containing polymer electrolyte systems such as PVdF-HFP-MG49  and PVdF-MG49  achieved the best ionic conductivity up to the order of 10−4 S cm−1 when blended with LiBF4 and LiCF3SO3, respectively. The polymer blend made up of PEO-MG49 reached the maximum conductivity from 4.0 × 10−9 S cm−1 to 8.0 × 10−6 S cm−1 upon addition of 15 wt.% LiClO4.
2.5. Interactions in MG-based polymer electrolytes
It is useful for researchers to investigate whether interactions have occurred between MG polymer and the salt, as well as with other components in the polymer electrolyte system, for example, plasticizer, filler, and so on, and identify the chemical group where the interactions have taken place. Interactions between components in a polymer electrolyte system will ensure miscibility and no phase separation.
As mentioned in previous sections, natural rubber does not possess polar atoms which could complex with cations from salt. In MG30 and MG49, the PMMA contains oxygen atoms in the C═O and C─O─C groups which have been reported to interact with the cations from salt through coordination bond(s) [4, 5, 20, 23, 24]. Evidence of complexation of MG30 and MG49 with various salts could be obtained from infrared (IR) spectroscopy. The wavenumber regions of interest of MG polymer matrices are ≈1720–1750 cm−1 and ≈950–1450 cm−1 which represent the C═O and C─O─C group, respectively. Shifting of the IR bands mentioned indicates complexation of MG polymer with cations from the salt.
Although interactions between MG polymer matrix and salt are usually shown from the shifting of the symmetrical C═O stretching (
Several reports on plasticized MG-based polymer electrolytes found no interaction from IR studies between the polymer matrix and the plasticizer. Kumutha and co-workers  reported on the IR analyses of MG30-LiCF3SO3-EC system and explored the interactions between MG30 and EC and between LiCF3SO3 and EC. For the MG30-EC sample, no IR change was found, which indicated that there was no interaction between the polymer and plasticizer. However, for the LiCF3SO3-EC mixture, the
Ali et al.  investigated on MG30-LiCF3SO3-PC system. The
In filler-added polymer electrolyte system, such as MG30-LiCF3SO3-EC-Al2SiO5, Kumutha et al.  did not observe any IR change to the spectra of polymer electrolyte upon incorporation of the filler. This indicates that Al2SiO5 did not interact with the components in the PE complex and only existed as dispersed solid.
The formation of MG49-PMMA blend was investigated by Ahmad et al.  using IR spectroscopy. The
For PEO-MG49-LiClO4 polymer blend electrolyte system, complexation between Li+ ions and the polymer blend was confirmed by Ahmad and co-workers  from the shifting of bands belonging to PEO and PMMA in MG49. The triple band due to PEO initially located at 1146, 1099, and 1060 cm−1 formed a single band in the range of 1066–1094 cm−1 in PEO-MG49-LiClO4 samples, which indicated coordination of Li+ ions on the O atoms in PEO. The
2.6. Determination of free ion, ion pairs and ion aggregates
Besides being able to reveal the interactions that occur in polymer electrolyte systems, IR analysis can also estimate the amount of charge carriers present in different samples. The result can be used to explain the conductivity behavior at different added contents of salt or other additives in the polymer electrolyte system.
Some IR regions representing certain bands of the salt could reveal the types of ionic species (i.e. free ions, ion pairs, ion aggregates) present and their area percentage in the polymer electrolytes. According to Huang and Frech , different types of triflate (CF3SO3−) ionic species can be distinguished from the deconvolution of the IR envelope of symmetrical stretching of SO3 (
Yap et al.  studied MG30 PE system added with varied LiCF3SO3 contents and noted the increase of conductivity up to 30 wt.% LiCF3SO3 with maximum conductivity of 1.7 µS cm−1 at 30°C before dropping beyond that composition. The IR spectra of LiCF3SO3, MG30, and MG30-LiCF3SO3 samples between 1000 and 1100 cm−1, where the
Yap and co-workers  reported the presence of free ions (1032 cm−1) and ion pairs (1040 cm−1) in the MG30-LiCF3SO3 samples. No ion aggregate was detected in the samples. The trend of free ions obeyed the trend of conductivity, whereby the highest area % of free ions was found in the best conducting sample, which is MG30 containing 30 wt.% LiCF3SO3. Increasing free ions with LiCF3SO3 contents is due to the recombination of Li+ and CF3SO3− ions. Hence, the trend of conductivity, that is, the rise of conductivity below 30 wt.% LiCF3SO3 and its subsequent drop above that composition was explained by the trend of free ions.
2.7. Determination of number density, mobility and diffusion coefficient values
By using the % area of free ions obtained from the IR deconvolution of
|LiCF3SO3 content (wt.%)||σ (S cm−1)||FI (%)|
|10||1.9 × 10−9||67.0||2.7 × 1022||4.3 × 10−13||1.1 × 10−14|
|20||1.1 × 10−8||70.0||6.0 × 1022||1.1 × 10−12||2.9 × 10−14|
|30||1.7 × 10−6||78.2||1.1 × 1023||10.0 × 10−11||2.6 × 10−12|
|40||6.4 × 10−8||68.6||1.3 × 1023||3.1 × 10−12||7.8 × 10−14|
Modified natural rubbers namely PMMA-grafted natural rubber (i.e. MG30 and MG49), are widely used as polymer matrices in polymer electrolytes. MG30 and MG49 contain polar C═O and C─O─C groups which could complex with cations from salt to produce ion transport. Plasticizers, such as EC, PC, DMC, and PEG200, were employed to enhance the conductivity of solid-based MG polymer matrices. Passive inorganic fillers, such as SiO2, Al2O3, TiO2, TiO2-SiO2, were used to improve the mechanical strength of the polymer electrolytes. Polymer blends of MG with PEO, PMMA, PVdF, and PVdF-HFP were able to improve the properties of MG-based polymer electrolytes in terms of conductivity and structural homogeneity. Complexation between MG polymer matrices and salt could usually be shown through IR shifts of bands corresponding to C═O and C─O─C groups, although in some cases, only changes in intensity were reported. Plasticizers and fillers added into MG polymer matrices did not manifest change on the IR spectra of the polymer, although interactions were found to occur between plasticizer and the salt (i.e., between LiCF3SO3 and EC or PC). MG30 and MG49-based polymer electrolytes could achieve high ionic conductivity up to 10-2 S cm-1 when plasticized and have potential to be used in electrochemical devices.
The authors would like to thank Ministry of Higher Education (MOHE) for grant FP053-2014A, SATU Joint Research Scheme RU022G-2014 and University of Malaya.
Fenton DE, Parker JM, Wright PV. Complexes of alkali metal ions with poly (ethylene oxide). Polymer. 1973; 14:589
Berthier C, Gorecki W, Minier M, Armand MB, Chabagno JM, Rigaud P. Microscopic investigation of ionic conductivity in alkali metal salts–poly(ethylene oxide) adducts. Solid State Ionics. 1983; 11:91-95
Kang OL, Ahmad A, Hassan NH, Rana UA. [MG49-LiClO4]:[TiO2-SiO2] polymer electrolytes: In situ preparation and characterization. International Journal of Polymer Science. 2016; 9838067
Ali AMM, Subban RHY, Bahron H, Yahya MZA, Kamisan AS. Investigation on modified natural rubber gel polymer electrolytes for lithium polymer battery. Journal of Power Sources. 2013; 244:636-640
Yap KS, Teo LP, Sim LN, Majid SR, Arof AK. Investigation on dielectric relaxation of PMMA-grafted natural rubber incorporated with LiCF3SO3. Physica B. 2012; 407:2421-2428
Santhosh P, Gopalan A, Vasudevan T, Lee KP. Evaluation of a cross-linked polyurethane acrylate as polymer electrolyte for lithium batteries. Materials Research Bulletin. 2006; 41:1023-1037
Wu N, Cao Q, Wang X, Li S, Li X, Deng H. In situ ceramic fillers of electrospun thermoplastic polyurethane/poly(vinylidene fluoride) based gel polymer electrolytes for Li-ion batteries. Journal of Power Sources. 2011; 196:9751-9756
Zhou L, Jing B, Wang X, Tang X, Wu N. Study of a novel porous gel polymer electrolyte based on thermoplastic polyurethane/poly(vinylidene fluoride-co-hexafluoropropylene) by electrospinning technique. Journal of Power Sources. 2014; 263:118-124
Yoshimoto N, Nomura H, Shirai T, Ishikawa M, Morita M. Ionic conductance of gel electrolyte using a polyurethane matrix for rechargeable lithium batteries. Electrochimica Acta. 2004; 50:275-279
Wen TC, Chen WC. Gelled composite electrolyte comprising thermoplastic polyurethane and poly(ethylene oxide) for lithium batteries. Journal of Power Sources. 2001; 92:139-148
Wen TC, Kuo HH, Gopalan A. The influence of lithium ions on molecular interaction and conductivity of composite electrolyte consisting of TPU and PAN. Solid State Ionics. 2002; 147:171-180
Song JY, Wang YY, Wan CC. Review of gel-type polymer electrolytes for lithium-ion batteries. Journal of Power Sources. 1999; 77:183-197
Kang Y, Lee W, Suh DH, Lee C. Solid polymer electrolytes based on cross-linked polysiloxane-g-oligo(ethylene oxide): Ionic conductivity and electrochemical properties. Journal of Power Sources. 2003; 119-121:448-453
Zhang ZC, Jin JJ, Bautista F, Lyons LJ, Shariatzadeh N, Sherlock D, Amine K, West R. Ion conductive characteristics of cross-linked network polysiloxane-based solid polymer electrolytes. Solid State Ionics. 2004; 170:233-238
Kang Y, Lee J, Suh DH, Lee C. A new polysiloxane based cross-linker for solid polymer electrolyte. Journal of Power Sources. 2005; 146:391-396
Cznotka E, Jeschke S, Wiemhofer H-D. Characterization of semi-interpenetrating polymer electrolytes containing poly(vinylidene fluoride-co-hexafluoropropylene) and ether-modified polysiloxane. Solid State Ionics. 2016; 289:35-47
Seidel SM, Jeschke S, Vettikuzha P, Wiemhofer HD. PVDF-HFP/ether-modified polysiloxane membranes obtained via airbrush spraying as active separators for application in lithium ion batteries. Chemical Communications. 2015; 51:12048-12051
Rohan R, Pareek K, Chen Z, Cai W, Zhang Y, Xu G, Gao Z, Cheng H. A high performance polysiloxane-based single ion conducting polymeric electrolyte membrane for application in lithium ion batteries. Journal of Materials Chemistry A. 2015; 3:20267-20276
Iijima T, Tyoguchi Y, Eda N. Quasi-solid organic electrolytes gelatinized with PMMA and their applications for lithium batteries. 1985; 53:619-623
Brown H. A molecular interpretation of the toughness of glassy polymers. Macromolecules. 1991; 24:2752-2756
Kumutha K, Alias Y, Said R. FTIR and thermal studies of modified natural rubber based polymer electrolytes. Ionics. 2005; 11:472-476
Kumutha K, Alias Y. FTIR spectra of plasticized grafted natural rubber-LiCF3SO3 electrolytes. Spectrochimica Acta Part A. 2006; 64:442-447
Ali AMM, Subban RHY, Bahron H, Winie T, Latif F, Yahya MZA. Grafted natural rubber-based polymer electrolytes: ATR-FTIR and conductivity studies. Ionics. 2008; 14:491-500
Su’ait MS, Ahmad A, Hamzah H, Rahman MYA. Effect of lithium salt concentrations on blended 49% poly(methyl methacrylate) grafted natural rubber and poly(methyl methacrylate) based solid polymer electrolyte. Electrochimica Acta. 2011; 57:123-131
Zaki NHM, Mahmud ZS, Yahya MZA, Ali AMM. Conductivity studies on 30% PMMA grafted NR-NH4CF3SO3 Gel Polymer Electrolytes. 2012 IEEE Symposium on Humanities, Science and Engineering Research. 2012; 6268995:797-800
Ali AMM, Yahya MZA, Bahron H, Subban RHY. Electrochemical studies on polymer electrolytes based on poly(methyl methacrylate)-grafted natural rubber for lithium polymer battery. Ionics. 2006; 12:303-307
Low SP, Ahmad A, Rahman MYA. Effect of ethylene carbonate plasticizer and TiO2 nanoparticles on 49% poly(methyl methacrylate) grafted natural rubber-based polymer electrolyte. Ionics. 2010; 16:821-826
Hashim H, Adam NI, Zaki NHM, Mahmud ZS, Said CMS, Yahya MZA, Ali AMM. Natural rubber-grafted with 30% poly(methylmethacrylate) characterization for application in lithium polymer battery. 2010 International Conference on Science and Social Research. 2010; 5773825:485-488
Yap KS, Teo LP, Sim LN, Majid SR, Arof AK. Plasticised polymer electrolytes based on PMMA grafted natural rubber-LiCF3SO3-PEG200. Materials Research Innovations. 2011; 15:34-38
Kamisan AS, Kudin TIT, Ali AMM, Yahya MZA. Electrical and physical studies on 49% methyl-grafted natural rubber-based composite polymer gel electrolytes. Electrochimica Acta. 2011; 57:207-211
Adam NI, Zaki NHM, Mahmud ZS, Yahya MZA. The effect of composition nanofiller Al2O3 to the conductivity, morphology and thermal properties of MG30-LiTf polymer electrolyte. IEEE Symposium on Business, Engineering and Industrial Applications. 2012; 6422980:701-704
Aziz AFB, Ali AMM. Thermal oxidation studies on methyl grafted natural rubber polymer electrolytes with paraphenylene diamine additive. 2012 IEEE Colloquium on Humanities, Science and Engineering Research. 2012; 6504406:719-723
Li GY, Koenig JL. FTIR imaging of oxidation of polyisoprene 2. The role of N-phenyl-Nƍ-dimethyl-butyl-p-phenylenediamine antioxidant. Polymer Degradation and Stability. 2003; 81:377-385
Narathichat M, Sahakaro K, Nakason C. Assessment degradation of natural rubber by moving die processability test and FTIR spectroscopy. Journal of Applied Polymer Science. 2010; 115:1702-1709
Su’ait MS, Ahmad A, Rahman MYA. Ionic conductivity studies of 49% poly(methyl methacrylate)-grafted natural rubber-based solid polymer electrolytes. Ionics. 2009; 15:497-500
Ahmad A, Rahman MYA, Su’ait MS, Hamzah H. Study of MG49-PMMA based polymer electrolyte. The Open Materials Science Journal. 2011; 5:170-177
Ataollahi N, Ahmad A, Hamzah H, Rahman MYA, Mohamed NS. Preparation and characterization of PVDF-HFP/MG49 based polymer blend electrolyte. International Journal of Electrochemical Science. 2012; 7:6693-6703
TianKhoon L, Ataollahi N, Hassan NH, Ahmad A. Studies of porous solid polymeric electrolytes based on poly(vinylidene fluoride) and poly(methyl methacrylate) grafted natural rubber for applications in electrochemical devices. Journal of Solid State Electrochemistry. 2016; 20:203-213
Ahmad A, Rahman MYA, Su’ait MS. Morphological, infrared, and ionic conductivity studies of poly(ethylene oxide)-49% poly(methyl methacrylate) grafted natural rubber-lithium perchlorate salt based solid polymer electrolytes. Journal of Applied Polymer Science. 2012; 124:4222-4229
Xi J, Qiu X, Zheng S, Tang X. Nanocomposite polymer electrolyte comprising PEO/LiClO4 and solid super acid: Effect of sulphated-zirconia on the crystallization kinetics of PEO. Polymer. 2005; 46:5702-5706
Abdullah M, Lenggoro W, Okuyama. Polymer electrolyte nanocomposites. In: Nalwa HS, editor. Encyclopedia Nanoscience and Nanotechnology. American Scientific Publishers; USA: American Scientific Publishers; 2004. p. 731
Huang W, Frech R. Dependence of ionic association on polymer chain length in poly(ethylene oxide)–lithium triflate complexes. Polymer. 1994; 35:235-242